Innovative Refractory Technology for Coreless ... Innovative Refractory Technology for Coreless...
Embed Size (px)
Transcript of Innovative Refractory Technology for Coreless ... Innovative Refractory Technology for Coreless...
Innovative Refractory Technology for Coreless Induction Furnaces
Gulab Patel*, Himanshu Bhardwaj**, Raj Mohan***
*Manager-Product Application (firstname.lastname@example.org | +91-9727755600), Allied Refractory Products India **Regional Sales Manager-North India (email@example.com | +91-9999943299), Allied Refractory Products India ***Regional Sales Manager-South India (firstname.lastname@example.org | +91-9790958269), Allied Refractory Products India
Abstract In recent years, there has been industry pressure to provide larger and more powerful coreless
induction furnaces for melting both iron and steel alloys. Production demands and electrical costs
have driven many foundries and steel mills to invest in larger, faster, and more flexible batch
melting furnaces. These technological advancements in induction furnaces have put a greater
demand on refractory suppliers to provide innovative advancements in both acid and neutral based
refractory for these applications. This paper will discuss a completely new generation of refractories and address care of structural
components, installation, sintering and optimal operation of coreless induction furnaces to
significantly improve the lining life. This reduces total melting costs while providing great
consistency in refractory lining performance. Specific case studies where new technology refractories have been used will be referenced, and an
overview of refractory properties and compositions that are best applied in specific melting
applications will be provided.
Silica‐Based Refractories for Iron and Steel Melting Silica‐based refractories have long been the standard for foundries using coreless furnaces to melt
iron and iron alloys. Traditional lining materials include a high purity silica aggregate with a boron‐
based, heat-set binder, generally in the form of either boron oxide or boric acid. In the past, this
binder was mixed on site at the foundry, prior to installation. Technological advancements then
allowed the binder additives to be pre‐mixed by the refractory producer and shipped to the foundry
in a ready‐to‐use form. Silica‐based refractories have essentially maintained the same composition
for the past several decades, with only minor design changes and mineral additions.
Figure 1 – Iron melting coreless furnace with silica lining
mailto:email@example.com%20%7C%20+91-9727755600 mailto:firstname.lastname@example.org%20%7C%20+91-9999943299 mailto:email@example.com%20%7C%20+91-9790958269
Silica-based linings have many advantages for the traditional foundry:
• Low cost mineral base (in comparison to alumina‐based/neutral refractories). • Non‐wetting to iron and to most iron slag compositions. • Excellent thermal expansion properties for batch melting operations, limiting metal
penetration through thermal cracks.
• Refractory-grade silica deposits are in multiple sites around the world.
• Silica‐based refractories can also be used in copper alloy melting furnaces and furnaces melting some grades of steel alloys.
While silica-based refractories have many advantages, there are some deficiencies in the product range:
• The silica grain can be reduced by some common alloying elements at metal melting temperatures.
• Rapid bottom erosion (known as elephant’s foot erosion) due to mechanical, chemical, and
thermal factors occurs during the production of ductile iron, limiting lining life.
• Naturally high acidity of silica results in chemical erosion of lining when exposed to basic
• Mineral transformation and subsequent expansion that occurs with silica (quartz
transformation to tridymite) around 870°C extends sinter time during startup.
Technological Advancement in Silica Linings
A new range of silica based lining materials (Reference Figure 1) has been developed utilizing
advanced large grain technology (ALGT). The material employs a grain size of up to 12 mm in
diameter, which is 60 to 100% larger than the maximum grain sizing of traditional silica-based
refractories. The increased grain sizing results in a substantial reduction in the total surface area of the
refractory grains, and combined with new binding technology, provides a more effective and repeatable
sinter process. Additional benefits of the new technology are as follows:
• Large grains provide better particle packing, resulting in increased installed density of the lining.
• Improved abrasion resistance in service at metal melting temperature. • Binder system designed for liquid sintering of larger furnaces.
Case Studies for Improved Silica Linings Foundry A operates 3 coreless furnaces with a capacity of 7 MT each. Installation utilizes traditional
form vibration and sintering is completed with liquid metal charging. This foundry produces normal
grades of iron, as well as special grades melted above 1600°C. This special iron production results in
rapid, unpredictable erosion in the bottom of the furnace.
Results at Foundry A: Silica linings with ALGT have been installed for the complete lining, resulting in
a 10 to 20% increase in lining life over traditional silica for regular iron production. However, for the high
temperature special iron alloy production, an increase of up to 50% has been achieved due to better
sintering properties and increased abrasion resistance of the ALGT silica lining in the taper and bottom
section of the furnace. Foundry B is a large automotive foundry melting traditional gray and ductile iron in medium frequency
coreless furnaces. The facility operates multiple 3 MT and 5 MT furnaces on a single 12-hour shift
resulting in daily thermal cycling of the lining. The foundry already achieves excellent lining results of
350 heats per lining with minor repairs to the floor, taper and top cap. Results at Foundry B: A silica lining with ALGT has been used for the complete lining, resulting in a record campaign of 675 heats with one minor patch of the floor and taper area. All furnace linings have been successfully converted to take advantage of the extended campaign life.
Structural components (Top and Bottom Blocks/Spout/Grout) of coreless induction furnace: To achieve consistent lining life of coreless induction furnaces, these play very important roles.
• A-Top/Bottom Blocks: Need to check every time before lining to make sure it has tightened properly and in good shape/condition.
Bad Condition of both top and bottom blocks (Reference Figure 2) directly affects the performance of lining life. If it is cracked and not tightened properly, it creates impact on lining during operation (tilting) and results in lining cracks and leads to metal fining in lining through cracks.
• B-Spout: Always Install the Spout before the main lining (Reference Figure 3/5/6). It is important to maintain the vertical plan Refractory, to allow free movement, minimizing cracks and penetrations below the spout.
Figure 2 - Bottom block cracked
Figure 5 - Installed Spout with SP 83CR Figure 6 - Installed Spout with A 7055
It is incorrect procedure to install the spout above the working lining (Reference Figure 4) which inhibits the free movement of the working lining and adds stress that results in cracks and metal penetration.
• C- Coil Grout: o Must be smooth and concentric to allow the lining to expand and contract freely and avoid hang
up of lining which leads to cracks and eventual metal fining. o Should be strong enough to hold well upon lining demolition o Before installing the refractory, make sure the grout is completely dry.
Figure 7 - New generation pigmented Coil Grout 563
Figure 3 - Correct Spout Installation Procedure Figure 4 - Incorrect Spout Installation Procedure
Pigmented grout (Reference Figure 7) gives a visual reference between the lining and the grout to avoid damage during manual removal of old refractory. Specially designed fine-grain products allow 100% use, low shrinkage after air set and require less water and demonstrate easy dry out and high strength.
• SLIP PLANE: Use a good quality SLIP PLANE between working lining and coil grout, i.e., Mica sheet (Reference Figure-8). The Mica sheet should be adhered properly to the grout; there should be no space between the mica sheet and grout. Secure the mica with quality adhesive tape. Never use adhesive like sodium silicate or fevicol to secure mica sheet with grout.
• FORM: One of the important components which plays a vital role in determining the lining life of the coreless furnace.
o Adequate thickness of form is preferred and varies as furnace capacity increases. o The form should be designed to maintain its integrity for as long as possible, avoiding
localized deformation (Reference Figure 9) which could impair the density and saturation of the metal or promote slag.
o A thin sheet former might be damaged before hot face formation, thus reducing lining life. This will be good enough for taking the vibrator.
Figure 8 - Mica Sheet Installation
Figure 9 - Deformation of Former
Refractory Alternatives in